- X-ray photoelectron spectroscopy
monochromaticXPS system.] X-ray photoelectron spectroscopy(XPS) is a quantitative spectroscopic technique that measures the elemental composition, empirical formula, chemical stateand electronic stateof the elements that exist within a material. XPS spectraare obtained by irradiating a material with a beam of aluminium or magnesium X-rays while simultaneously measuring the kinetic energy(KE) and number of electronsthat escape from the top 1 to 10 nm of the material being analyzed. XPS requires ultra-high vacuum (UHV) conditions.
XPS is a surface chemical analysis technique that can be used to analyze the surface chemistry of a material in its "as received" state, or after some treatment such as: fracturing, cutting or scraping in air or UHV to expose the bulk chemistry, ion beam etching to clean off some of the surface contamination, exposure to heat to study the changes due to heating, exposure to reactive gases or solutions, exposure to ion beam implant, exposure to
ultraviolet light, for example.
* XPS is also known as ESCA, an abbreviation for Electron Spectroscopy for Chemical Analysis.
* XPS detects all elements with an
atomic number("Z") of 3 ( lithium) and above. This limitation means that it cannot detect hydrogen("Z"=1) or helium("Z"=2).
Detection limits for most of the elements are in the parts per thousandrange. Detections limits of parts per million(ppm) are possible, but require special conditions: concentration at top surface or very long collection time (overnight).
* XPS is routinely used to analyze
inorganic compounds, metal alloys, semiconductors, polymers, elements, catalysts, glasses, ceramics, paints, papers, inks, woods, plant parts, make-up, teeth, bones, medical implants, bio-materials, viscous oils, glues, ion modified materials and many others.
XPS is used to measure:
* elemental composition of the surface (1–10 nm usually)
empirical formulaof pure materials
* elements that contaminate a surface
* chemical or electronic state of each element in the surface
* uniformity of elemental composition across the top surface (aka, line profiling or mapping)
* uniformity of elemental composition as a function of ion beam etching (aka, depth profiling)
XPS can be performed using either a commercially built XPS system, a privately built XPS system or a
Synchrotron-based light source combined with a custom designed electron analyzer. Commercial XPS instruments in the year 2005 used either a highly focused 20 to 200 micrometer beam of monochromaticaluminium K-alpha X-rays or a broad 10-30 mm beam of non-monochromatic ( polychromatic) magnesium X-rays. A few, special design XPS instruments can analyze volatile liquids or gases, materials at low or high temperatures or materials at roughly 1 torrvacuum, but there are relatively few of these types of XPS systems.
Because the energy of a particular X-ray wavelength equals a known quantity, we can determine the
electron binding energy(BE) of each of the emitted electrons by using an equation that is based on the work of Ernest Rutherford(1914):
:"E"binding = "E"photon - "E"kinetic - "Φ"
where "E"binding is the energy of the electron emitted from one electron configuration within the atom, "E"photon is the energy of the X-ray photons being used, "E"kinetic is the kinetic energy of the emitted electron as measured by the instrument and "Φ" is the
work functionof the spectrometer (not the material).
History of XPS
Heinrich Rudolf Hertzdiscovered the photoelectric effect. Twenty years later, in 1907, P.D. Innes experimented with a Röntgentube, Helmholtz coils, a magnetic field hemisphere (electron energy analyzer) and photographic plates to record broad bands of emitted electrons as a function of velocity, in effect recording the first XPS spectrum. Other researchers, Moseley, Rawlinson and Robinson, independently performed various experiments trying to sort out the details in the broad bands. Due to the wars, research on XPS came to a halt. After WWII, Kai Siegbahnand his group in Sweden developed several significant improvements in the equipment and in 1954 recorded the first high energy resolution XPS spectrum of cleaved sodium chloride(NaCl) revealing the potential of XPS. A few years later in 1967, Siegbahn published a comprehensive study on XPS bringing instant recognition of the utility of XPS. In cooperation with Siegbahn, Hewlett-Packardin the USA produced the first commercial monochromatic XPS instrument in 1969. Siegbahn received the Nobel Prizein 1981 to acknowledge his extensive efforts to develop XPS into a useful analytical tool.
In parallel with Siegbahn's work, David Turner at Imperial College (and later at Oxford) in the UK developed
ultraviolet photoelectron spectroscopy(UPS) on molecular species using helium lamps.
Physics of XPS
A typical XPS spectrum is a plot of the number of electrons detected (Y-axis, ordinate) versus the
binding energyof the electrons detected (X-axis, abscissa). Each element produces a characteristic set of XPS peaks at characteristic binding energyvalues that directly identify each element that exist in or on the surface of the material being analyzed. These characteristic peaks correspond to the electron configurationof the electrons within the atoms, e.g., 1s, 2s, 2p, 3s, etc. The number of detected electrons in each of the characteristic peaks is directly related to the amount of element within the area (volume) irradiated. To generate atomic percentage values, each raw XPS signal must be corrected by dividing its signal intensity (number of electrons detected) by a "relative sensitivity factor" (RSF) and normalized over all of the elements detected.
To count the number of electrons at each KE value, with the minimum of error, XPS must be performed under
ultra-high vacuum(UHV) conditions because electron counting detectors in XPS instruments are typically one meter away from the material irradiated with X-rays.
It is important to note that XPS detects only those electrons that have actually escaped into the vacuum of the instrument. The photo-emitted electrons that have escaped into the vacuum of the instrument are those that originated from within the top 10 to 12 nm of the material. All of the deeper photo-emitted electrons, which were generated as the X-rays penetrated 1–5 micrometers of the material, are either recaptured or trapped in various excited states within the material. For most applications, it is, in effect, a non-destructive technique that measures the surface chemistry of any material.
Components of an XPS system
The main components of a commercially made XPS system include:
*A source of X-rays
*An ultra-high vacuum (
UHV) stainless steel chamber with UHV pumps
*An electron collection lens
*An electron energy analyzer
Mu-metalmagnetic field shielding
*An electron detector system
*A moderate vacuum sample introduction chamber
*A sample stage
*A set of stage manipulators
Monochromatic aluminium K-alpha X-rays are normally produced by diffracting and focusing a beam of non-monochromatic X-rays off of a thin disc of natural, crystalline
quartzwith a <1010> lattice. The resulting wavelength is 8.3386 angstroms (0.83386 nm) which corresponds to a photon energy of 1486.7 eV. The energy width of the monochromated X-rays is 0.16 eV, but the common electron energy analyzer (spectrometer) produces an ultimate energy resolution on the order of 0.25 eV which, in effect, is the ultimate energy resolution of most commercial systems. When working under practical, everyday conditions, high energy resolution settings will produce peak widths (FWHM) between 0.4-0.6 eV for various pure elements and some compounds.
Non-monochromatic magnesium X-rays have a wavelength of 9.89 angstroms (0.989 nm) which corresponds to a photon energy of 1253 eV. The energy width of the non-monochromated X-ray is roughly 0.70 eV, which, in effect is the ultimate energy resolution of a system using non-monochromatic X-rays. Non-monochromatic X-ray sources do not use any crystals to diffract the X-rays which allows all primary X-rays lines and the full range of high energy
BremsstrahlungX-rays (1–12 keV) to reach the surface. The typical ultimate high energy resolution (FWHM) when using this source is 0.9–1.0 eV, which includes with the spectrometer-induced broadening, pass-energy settings and the peak-width of the non-monochromatic magnesiumX-ray source.
Uses and capabilities
XPS is routinely used to determine:
* What elements and the quantity of those elements that are present within ~10 nm of the sample surface
* What contamination, if any, exists in the surface or the bulk of the sample
* Empirical formula of a material that is free of excessive surface contamination
* The chemical state identification of one or more of the elements in the sample
* The binding energy (BE) of one or more electronic states
* The thickness of one or more thin layers (1–8 nm) of different materials within the top 10 nm of the surface
* The density of electronic states
Capabilities of advanced systems
* Measure uniformity of elemental composition across the top the surface (aka, line profiling or mapping)
* Measure uniformity of elemental composition as a function of depth by ion beam etching (aka, depth profiling)
* Measure uniformity of elemental composition as a function of depth by tilting the sample (aka, angle resolved XPS)
Industries that use XPS
Adhesion, Agriculture, Automotive, Battery, Beverage, Biotech, Canning, Catalyst, Ceramic, Chemical, Computer, Cosmetic, Electronics, Environmental, Fabrics, Food, Fuel cells, Geology, Glass, Laser, Lighting, Lubrication, Magnetic memory, Mineralogy, Mining, Nuclear, Packaging, Paper and wood, Plating, Polymer and plastic, Printing, Recording, Semiconductor, Steel, Textiles, Thin-film coating, Welding
Routine limits of XPS
* Quantitative accuracy depends on several parameters such as: S/N, peak intensity, accuracy of relative sensitivity factors, correction for electron transmission function, surface volume homogeneity, correction for energy dependency of electron mean free path, and degree of sample degradation due to analysis.
* Under optimum conditions, the quantitative accuracy of the atom % values calculated from the Major XPS Peaks is 90-95% of the atom % values of each major peak. If a high level quality control protocol is used, the accuracy can be further improved.
* Under routine work conditions, where the surface is a mixture of contamination and expected material, the accuracy ranges from 80-90% of the value reported in atom % values.
* The quantitative accuracy for the weaker XPS signals, that have peak intensities 10-20% of the strongest signal, are 60-80% of the true value.
* 1–10 minutes for a survey scan that measures the amount of all elements, 1–10 minutes for high energy resolution scans that reveal chemical state differences, 1–4 hours for a depth profile that measures 4–5 elements as a function of etched depth (usual final depth is 1,000 nm)
* 0.1–1.0 atom % (0.1 atom% = 1 part per thousand = 1,000 ppm). (Ultimate detection limit for most elements is approximately 100 ppm, which requires 8–16 hours.)
Analysis area limits
* Analysis area depends on instrument design. The minimum analysis area ranges from 10 to 200 micrometres. Largest size for a monochromatic beam of X-rays is 1–5 mm. Non-monochromatic beams are 10–50 mm in diameter. Spectroscopic image resolution levels of 200 nm or below has been achieved on latest imaging XPS instruments using synchrotron radiation as X-ray source.
ample size limits
* Older instruments accept samples: 1x1 to 3x3 cm. Very recent systems can accept full 300 mm wafers and samples that are 30x30 cm.
Degradation during analysis
* Depends on the sensitivity of the material to the wavelength of X-rays used, the total dose of the X-rays, the temperature of the surface and the level of the vacuum. Metals, alloys, ceramics and most glasses are not measurably degraded by either non-monochromatic or monochromatic X-rays. Some, but not all, polymers, catalysts, certain highly oxygenated compounds, various inorganic compounds and fine organics are degraded by either monochromatic or non-monochromatic X-ray sources.
* Non-monochromatic X-ray sources produce a significant amount of high energy Bremsstrahlung X-rays (1–15 keV of energy) which directly degrade the surface chemistry of various materials. Non-monochromatic X-ray sources also produce a significant amount of heat (100 to 200 °C) on the surface of the sample because the anode that produces the X-rays is typically only 1 to 5 cm away from the sample. This level of heat, when combined with the Bremsstrahlung X-rays, acts synergistically to increase the amount and rate of degradation for certain materials. Monochromatic X-ray sources, because they are far away (50–100 cm) from the sample, do not produce any heat effects. Monochromatic X-ray sources are monochromatic because the quartz monochromator system diffracted the Bremsstrahlung X-rays out of the X-ray beam which means the sample only sees one X-ray energy, for example: 1.486 keV if aluminium K-alpha X-rays are used.
* Because the vacuum removes various gases (eg O2, CO) and liquids (eg water, alcohol, solvents) that were initially trapped within or on the surface of the sample, the chemistry and morphology of the surface will continue to change until the surface achieves a steady state. This type of degradation is sometimes difficult to detect.
Materials routinely analyzed by XPS
Inorganic compounds, metal alloys, semiconductors, polymers, pure elements, catalysts, glasses, ceramics, paints, papers, inks, woods, plant parts, make-up, teeth, bones, human implants, bio-materials, viscous oils, glues, ion modified materials
Organic chemicals are not routinely analyzed by XPS because they are readily degraded by the either the energy of the X-rays or the heat from non-monochromatic X-ray sources.
Charge compensation techniques
* Low Voltage Electron Beam (1-20 eV) [aka Electron Flood Gun]
* UV light
* Low Voltage Argon Ion Beam with Low Voltage Electron Beam (1-10 eV)
* Aperture mask
* Mesh screen with Low Voltage Electron Beam
* Sample handling
* Sample cleaning
* Sample mounting
Charge referencing insulators
* Using C 1s BE of hydrocarbon components (moieties)
* Typical FWHM
Ultra-violet photoelectron spectroscopy(for gases, aka PES)
Photoemission spectroscopy(for solid surfaces, aka UPS)
Zero Electron Kinetic Energyspectroscopy
Auger electron spectroscopy(AES)
* "Annotated Handbooks of Monochromatic XPS Spectra, PDF of Volumes 1 and 2", B.V.Crist, published by XPS International LLC, 2005, Mountain View, CA, USA
* "Handbooks of Monochromatic XPS Spectra, Volumes 1-5", B.V.Crist, published by XPS International LLC, 2004, Mountain View, CA, USA
* "Surface Analysis by Auger and X-ray Photoelectron Spectroscopy", ed. J.T.Grant and D.Briggs, published by IM Publications, 2003, Chichester, UK
* "Practical Surface Analysis by Auger and X-ray Photoelectron Spectroscopy", 2nd edition, ed. M.P.Seah and D.Briggs, published by Wiley & Sons, 1992, Chichester, UK
* "Practical Surface Analysis by Auger and X-ray Photoelectron Spectroscopy", ed. M.P.Seah and D.Briggs, published by Wiley & Sons, 1983, Chichester, UK ISBN 0-471-26279-X
* "Surface Chemical Analysis -- Vocabulary", ISO 18115 : 2001,
International Organisation for Standardisation(ISO), TC/201, Switzerland, [http://www.iso.ch]
* "Handbook of X-ray Photoelectron Spectroscopy", J.F.Moulder, W.F.Stickle, P.E.Sobol, and K.D.Bomben, published by Perkin-Elmer Corp., 1992, Eden Prairie, MN, USA
* "Handbook of X-ray Photoelectron Spectroscopy", C.D.Wagner, W.M.Riggs, L.E.Davis, J.F.Moulder, and G.E.Mullenberg, published by Perkin-Elmer Corp., 1979, Eden Prairie, MN, USA
Ultra-violet photoelectron spectroscopy
List of materials analysis methods
Wikimedia Foundation. 2010.
См. также в других словарях:
X-ray photoelectron spectroscopy — rentgeno fotoelektroninė spektroskopija statusas T sritis chemija apibrėžtis Spektroskopijos metodas, kai bandinys apšviečiamas monochromatiniais rentgeno spinduliais, sukeliančiais elektronų emisiją iš X ray photoelectron spectroscopy 3 nm… … Chemijos terminų aiškinamasis žodynas
X-ray photoelectron spectroscopy — X ray Photoelectron Spectroscopy (XPS), Electron Spectroscopy for Chemical Analysis (ESCA) Рентгеновская фотоэлектронная спектроскопия, РФЭС Метод анализа поверхности, основанный на регистрации энергетических спектров электронов,… … Толковый англо-русский словарь по нанотехнологии. - М.
X-ray photoelectron spectroscopy — fotoelektroninė rentgeno spektroskopija statusas T sritis radioelektronika atitikmenys: angl. X ray photoelectron spectroscopy vok. Röntgenphotoelektronenspektroskopie, f rus. рентгеновская фотоэлектронная спектроскопия, f pranc. spectroscopie… … Radioelektronikos terminų žodynas
Ultraviolet photoelectron spectroscopy — (UPS) refers to the measurement of kinetic energy spectra of photoelectrons emitted by ultraviolet photons, to determine molecular energy levels in the valence region.If Einstein’s photoelectric law is applied to a free molecule, the kinetic… … Wikipedia
X-ray photoelectron spectrometry — Spectrométrie de fluorescence X Pour les articles homonymes, voir SFX, FX et XRF. Un spectromètre de fluorescence X Philips PW1606 avec manutention automatiq … Wikipédia en Français
Spectroscopy — Analysis of white light by dispersing it with a prism is example of spectroscopy. Spectroscopy ( … Wikipedia
spectroscopy — spectroscopist /spek tros keuh pist/, n. /spek tros keuh pee, spek treuh skoh pee/, n. the science that deals with the use of the spectroscope and with spectrum analysis. [1865 70; SPECTRO + SCOPY] * * * Branch of analysis devoted to identifying… … Universalium
Auger electron spectroscopy — (AES; Auger pronounced|oːʒeː in French) is a common analytical technique used specifically in the study of surfaces and, more generally, in the area of materials science. Underlying the spectroscopic technique is the Auger effect, as it has come… … Wikipedia
Photoemission spectroscopy — (PES), also known as photoelectron spectroscopy, refers to energy measurement of electrons emitted from solids, gases or liquids by the photoelectric effect, in order to determine the binding energies of electrons in a substance. The term refers… … Wikipedia
Electron spectroscopy — is an analytical technique to study the electronic structure and its dynamics in atoms and molecules. In general an excitation source such as x rays, electrons, or synchrotron radiation will eject an electron from an inner shell orbital of an… … Wikipedia